This paper discusses a theoretical approach towards synthesizing broadband circularly polarizing reflectors. The broadband polarizing reflectors consist of birefringent metallo-dielectric metasurfaces which are described by the Jones matrices and verified via full-wave simulations. Specifically, full-wave simulations for candidate designs are presented that target operation in the near infrared band. In addition, reconfigurability is introduced and demonstrated for candidate designs at the long wave infrared band through the inclusion of a bistable phase change chalcogenide glass substrate.
©2013 Optical Society of America
Electromagnetic metamaterials are engineered structures that utilize periodic sub-wavelength patterning to create an effective macroscopic response. The engineered resonances and symmetries of the metamaterial can mimic or facilitate behavior not found in naturally occurring materials [1,2]. Each unit cell is most commonly comprised of a planarized metallic inductor - capacitor (LC) resonant circuit along with a supporting low loss dielectric substrate. This approach, with the appropriate geometry scaling, allows metamaterials to be applied to radio waves, microwaves, terahertz waves, and even into the infrared and optical ranges where fabrication constraints and ohmic losses can become a limiting factor. The metamaterial unit cell geometry is generally treated as a flat (d = λ), two-dimensional periodic surface with a sub-wavelength unit cell width (w ˂ λ). As a result, propagation distance through the dielectric can generally be ignored, and diffraction is eliminated at normal incidence in addition to a considerable range of oblique angles. Metamaterials can be considered to be weakly spatially dispersive, due to the small periodicity of the unit cells compared to the characteristic wavelength. Thus, due to a reduced field interaction, the sub-wavelength design requires that an efficient, and in turn high Q-factor, LC-type resonator be employed, the most familiar of which is the split ring resonator (SRR) .
Recently, interest is transitioning from the inherent narrowband behavior of LC resonators to metamaterials that exhibit broadband behavior. Broadband metamaterial design methodologies represent an emerging technology with a wide range of potential applications [4–8]. For example, they can be utilized in conjunction with existing communication bands or designed to coincide with atmospheric transmission windows. In this paper, a theoretical analysis is presented on the synthesis of broadband circularly polarizing mirrors. Full wave simulations are performed on candidate designs with traditional dielectric substrates in addition to designs which incorporate bistable phase changing substrates, facilitating broadband polarization reconfigurability.
2. Scattering from a two dimensional infinitely periodic metamaterial
Let us assume that a planar metamaterial is infinitely periodic along the X - Y plane. A forward traveling plane wave propagates along a vector at an angle, θ, off surface normal and subsequently interacts with the metamaterial. This interaction, or more specifically the linear, lossless scattering of polarized light, can be described in a manner similar to Jones matrix calculus [9–13] as described elsewhere . The forward propagating transmission matrix is given as:14]:14]. Therefore, if the incident vector is rotated 180° around the Y axis, the resultant scattering matrix, as a function of the original scattering parameters, is given by the backwards scattering matrix:Eq. (4) results in ,
Next, in the absence of any static magnetic fields, we can apply the Lorentz reciprocity theorem . When applied to oppositely propagating vectors the Lorentz reciprocity theorem results in the following scattering relationship:Eq. (7) results in ,Eqs. (10-11) hold in addition to:16]:Eq. (4) and Eq. (7), we can understand the scattering properties of a planar reciprocal metamaterial for a single plane of incidence and three related directions. Their relationships are summarized in Fig. 1 .
Solving for the scattering matrix coefficients, the forward and backward scattering eigenvalues,, are determined as follows:14]. As a result, the eigenvalues reduce to:17]:14]:Eq. (22) implies that Returning to Eq. (17), we have:Eq. (1) can now be expressed as,Eq. (25) is satisfied for azimuthal rotations measured between the incident field and the metamaterial line of symmetry which satisfy Therefore, Eq. (25) can be expressed in terms of under these bounds as,
To demonstrate the polarization conversion of the birefringent metamaterial, a normally incident plane wave,Fig. 2 ).
With an additional azimuthal rotation, the reflection can be considered as maximized or minimized respectively. In other words, the metamaterial does not couple with the electric field for but, it becomes resonantly excited for Thus, a planar electrically resonant anisotropic metamaterial can be represented as:Eqs. (19), (29) that the maximum circularly polarized reflection which can occur with a birefringent metamaterial structure is 50% of the incident field power. Yet, intuition applied to the equivalent surface impedance (Eq. (32)) provides a solution for 100% CP reflection. Specifically, creating a composite structure by backing it with a metallic ground plane such that:18].
Alternatively, this can be explained by first recognizing that the incident linearly polarized plane wave can be decomposed into two co-propagating CP waves of opposite handedness. Next, the result of Eq. (30) reveals that the transmission eigenstate for the metamaterial is . Applying Eq. (4), the transmission eigenstate for reverse propagation is which also happens to represent the transmitted field after reflection from the ground plane. In such a configuration, where the field transmits through the metamaterial and reflects off a ground plane, the field propagates through the dielectric substrate with negligible net phase advancement and retransmits through the now transparent metamaterial, resulting in the following transmission matrix:Fig. 3 ),
The propagation is phase-delayed due to the inductance attributed to the finite substrate transmission line length, wherein a properly tuned structure will have a total phase advancement of zero degrees for the round-trip wave propagation through the dielectric [19,20].
The reflection of the composite metasurface can alternatively be described for all azimuthal angles through the use of Jones calculus applied to rotational polarization elements [9–13]. Where, at normal incidence, the metasurface reflection matrix is:Eq. (33). As demonstrated with the matrices given by Eqs. (1-3), the metasurface reflection matrix is extended to oblique angles of incidence where reasonable agreement is assumed for a considerable field of view (FOV),
At this juncture, several assumptions have been utilized in order to simplify the analysis. For example, a 2D infinite periodic structure has been assumed for simulation purposes. Such an assumption is commonly expected to agree with physical measurements if the metamaterial structure has an overall dimension of several wavelengths in both directions. Additionally, the assumption of a negligible substrate thickness has been refined to be that of insignificant electrical distance. However, the assumption of low loss needs further consideration. For example, Eq. (31) is only partially valid since loss is not taken into account. The well-known Kramers-Kronig relations,21]. Fortunately, this loss is generally much smaller than the reactance slightly off resonance; thus, a simple solution for metamaterial design is to work in this lower loss frequency region. Nevertheless, Eq. (40) is essentially valid for a solitary frequency point since negative permittivity is a resonance induced phenomenon and in turn highly dispersive. As a result, broadband planar metamaterials are inherently challenging.
3. Broadband circularly polarizing metasurfaces
As previously discussed, the desire for broadband metamaterials is primarily driven by existing communication bands and atmospheric transmission windows. Revisiting Eq. (40), it will now be shown that this condition can exist in between two resonances if the resonances are sufficiently separated in frequency and occur along orthogonal axes. In turn, the resulting dispersive N matrix supporting broadband CP reflection is given by:Eq. (40), can still be utilized when Eq. (28) to Eq. (47), the reflected wave may be expressed in the form:Eq. (48) is readily achieved over a considerable bandwidth when the two frequency offset orthogonal resonances are low loss and have comparable Q factors.
3.1 Broadband infrared circularly polarizing metasurface simulation and performance metrics
To validate Eq. (48) and emphasize the advantages of metamaterials, two examples are presented for the short wave infrared band, using full wave simulations with dispersive material parameters measured via ellipsometry. To simultaneously convey the reflected wave intensity, bandwidth and polarization, the Stokes parameters are utilized . The Stokes vector is represented by the I (intensity), Q (linear polarization), U (45 degree rotated linear polarization) and V (circular) parameters. In Cartesian coordinates, the Stokes parameters are calculated as follows:
The first metallo-dielectric structure is a 2D infinitely periodic metasurface that consists of capacitively end-loaded dipole elements. The unit cell is 480 nm x 480 nm and the dipole is comprised of 75 nm thick Au, supported by a 75 nm polyimide substrate, and backed by a 200 nm Au ground plane. The lower resonance, , caused by the decomposition of an incident linear wave parallel to the dipole axis falls into the realm of metamaterial (i.e. sub-wavelength) behavior due to the size reduction caused by the capacitive end-loading of adjacent unit cells. However, the orthogonal resonance, , does not occur at a sufficiently large wavelength because it is attributed to the formation of a dependent grating which is in turn highly angularly dependent . Consequently, a very broadband CP design is achieved at normal incidence but performance degrades rapidly for increasing oblique angles (Fig. 4(a) ), limiting the utility of the design.
The second metallo-dielectric structure is a 2D infinitely periodic metasurface that consists of split ring (SR) elements. The unit cell is 380 nm x 380 nm and the SR is comprised of 75 nm thick Au, supported by a 50 nm Polyimide substrate, and backed by a 200 nm Au ground plane. The lower resonance, , is caused by the decomposition of an incident linear wave perpendicular to the SR gap. The upper orthogonal resonance is a caused by the decomposition of an incident linear wave parallel to the SR gap. Both resonances fall within the realm of metamaterial behavior due to the retention of a sufficiently sub wavelength geometry at both frequencies. This directly results in a broadband CP reflector with a wide field of view (FOV). Referencing Fig. 4(b), a low loss, wide FOV, wide CP band centered at λ = 1.55 µm is evident.
For added clarity the SR metasurface polarization response for a horizontally polarized wave normally incident upon a rotated SR metasurface is represented by additional metrics in Fig. 5 The metrics utilized are axial ratio and polarization conversion ratio (PCR) respectively. These metrics are useful in comparing the published performance for metamaterial based polarizers presented elsewhere across various spectrum [24–34] in addition to conventional dielectric quarter wave plates. Figure 6(a) depicts the complete Stokes parameters at normal incidence and Fig. 6(b) depicts the complete Stokes parameters for as a function of a normally incident field’s azimuthal rotation.
3.2 Broadband reconfigurable circularly polarizing metasurface using phase change materials
The utility of the circularly polarizing metasurface can be increased if reconfigurability is introduced since polarization sensing can offer a lower signal to noise ratio than amplitude modulation. Some examples of reconfigurable metamaterials include the incorporation of a semiconducting substrate  or inclusion of a semiconducting device [36,37], the incorporation of cantilevers [38,39] or MEMs , and the incorporation of phase change materials (PCM) [39–42]. Chalcogenide glass (ChG) PCMs have gained considerable interest due to their reversible, thermally-induced phase transition between amorphous and crystalline states with a large associated change in electrical and optical properties .
To demonstrate the effect of upper and lower resonance Q factor symmetry and unit cell size, three examples are presented for the long wave infrared band. Each design incorporates a Ge2Sb2Te5 (GST) ChG PCM substrate and functions as a circular polarizer when the GST is in the amorphous state. In the crystalline state the substrate becomes lossy, resulting in a mirror like reflection with no polarization conversion. The measured values utilized for GST at λ = 10µm are n = 4.2, k = 0.01 in the amorphous state and n = 8, k = 4.8 in the crystalline state. As with the near IR designs, full wave simulations consider all losses using material parameters measured via ellipsometry.
The first metallo-dielectric structure is a 2D infinitely periodic metasurface that consists of end-loaded dipole elements. The unit cell is 700 nm x 700 nm and the dipole is comprised of 150 nm thick Au, supported by a 430 nm GST substrate, and backed by a 150 nm Au ground plane. The lower resonance, , is caused by the decomposition of an incident linear wave parallel to the dipole axis. The orthogonal resonance, , is attributed to the higher Q end load resonance. Since the structure is sufficiently sub-wavelength, good angular performance is exhibited (Fig. 7(a) ); but, the asymmetrical Q factors result in a reduced region of high CP.
The second metallo-dielectric structure is a 2D infinitely periodic metasurface that consists of meander line elements. The unit cell is 900 nm x 1800 nm and the meander line is comprised of 150 nm thick Au, supported by a 400 nm GST substrate, and backed by a 150 nm Au ground plane. While exhibiting a broad bandwidth and reasonably comparable Q factors for the lower and upper resonances (Fig. 7(b)), the large unit cell length results in a deterioration of angular performance. This is exhibited by the emergence of an in-band resonance at larger oblique angles.
The third metallo-dielectric structure is the familiar SR design with appropriate geometry scaling. The unit cell is 975 nm x 975 nm and the SR is comprised of 150 nm thick Au, supported by a 465 nm GST substrate, and backed by a 150 nm Au ground plane. Since the structure is sufficiently sub-wavelength and exhibits highly symmetric Q factors, broad bandwidth and good angular performance is exhibited (Fig. 7(c)). Furthermore, when the GST substrate phase is changed to the crystalline state the structure no longer behaves as a broadband birefringent surface but rather as a metallic mirror (Fig. 7(d)).
A theoretical analysis utilizing Jones matrices is presented, enabling the synthesis of broadband circularly polarizing mirrors. The theoretical analysis and the validity of the associated assumptions are confirmed through full wave simulations performed on candidate designs with traditional dielectric substrates in addition to designs which incorporate the bistable phase changing substrate GST, facilitating broadband polarization reconfigurability.
References and links
1. V. G. Veselago, “The electrodynamics of substances with simultaneously negative value of ε and μ,” Sov. Phys. Usp. 10(4), 509–514 (1968). [CrossRef]
3. J. B. Pendry, A. J. Holden, D. J. Robbins, and W. J. Stewart, “Magnetism from conductors and enhanced nonlinear phenomena,” IEEE Trans. Microw. Theory Tech. 47(11), 2075–2084 (1999). [CrossRef]
5. Z. H. Jiang, M. D. Gregory, and D. H. Werner, “Experimental demonstration of a broadband transformation optics lens for highly directive multibeam emission,” Phys. Rev. B 84(16), 165111 (2011). [CrossRef]
6. Z. H. Jiang, M. D. Gregory, and D. H. Werner, “A broadband monopole antenna enabled by an ultra-thin anisotropic metamaterial coating,” IEEE Antennas Wirel. Propag. Lett. 10, 1543–1546 (2011). [CrossRef]
7. Z. H. Jiang, Q. Wu, and D. H. Werner, “Demonstration of enhanced broadband unidirectional electromagnetic radiation enabled by a subwavelength profile leaky anisotropic zero-index metamaterial coating,” Phys. Rev. B 86(12), 125131 (2012). [CrossRef]
8. Q. Wu, C. P. Scarborough, D. H. Werner, E. Lier, and X. Wang, “Design synthesis of metasurfaces for broadband hybrid-mode horn antennas with enhanced radiation pattern and polarization characteristics,” IEEE Trans. Antenn. Propag. 60(8), 3594–3604 (2012). [CrossRef]
9. C. R. Jones, “A new calculus for the treatment of optical systems. I. Description and discussion of the calculus,” J. Opt. Soc. Am. 31(7), 488–493 (1941). [CrossRef]
10. C. R. Jones, “A new calculus for the treatment of optical systems. VI. Experimental determination of the matrix,” J. Opt. Soc. Am. 37(2), 110–112 (1947). [CrossRef]
11. C. R. Jones, “A new calculus for the treatment of optical systems. VII. Properties of the N-matricies,” J. Opt. Soc. Am. 38(8), 671–685 (1948). [CrossRef]
12. C. R. Jones, “New calculus for the treatment of optical systems. VIII. Electromagnetic theory,” J. Opt. Soc. Am. 46(2), 126–131 (1956). [CrossRef]
13. E. Collett, “Field guide to polarization,” in SPIE Field Guides, J.E. Greivenkamp, ed. (SPIE, 2005), Vol. FG05.
14. A. A. Maradudin, Structured Surfaces as Optical Metamaterials (Cambridge University Press, 2011).
15. J. Kong, Electromagnetic Wave Theory (Wiley, 1986).
16. V. Lindell, A. H. Sihvola, S. A. Tretyakov, and A. J. Viitanen, Electromagnetic Waves in Chiral and Bi-Isotropic Media (Artech House, 1994).
17. E. Plum, Chirality and Metamaterials (Ph.D. Thesis, University of Southampton, 2010).
18. P. E. Sieber and D. H. Werner, “A reconfigurable near-infrared circularly polarizing reflector based on phase changing anisotropic metamaterials,” Proceedings of the International Symposium on Antennas and Propagation and USNC/URSI National Radio Science Meeting (IEEE, 2012), IF54.2.
19. F. Costa, A. Monorchio, and G. Manara, “Analysis and design of ultra thin electromagnetic absorbers comprising resistively loaded high impedance surfaces,” IEEE Trans. Antenn. Propag. 58(5), 1551–1558 (2010). [CrossRef]
20. N. Behdad, M. Al-Joumayly, and M. Salehi, “A low-profile third-order bandpass frequency selective surface,” IEEE Trans. Antenn. Propag. 57(2), 460–466 (2009). [CrossRef]
21. T. H. Hand, Design and Applications of Frequency Tunable and Reconfigurable Metamaterials. (Ph.D. Thesis, Duke University, 2009).
22. C. H. Papas, Theory of Electromagnetic Wave Propagation (McGraw-Hill, 1965).
23. B. Munk, Frequency Selective Surfaces: Theory and Design (Wiley, 2000).
24. D. S. Lerner, “A wave polarization converter for circular polarization,” IEEE Trans. Antenn. Propag. 13(1), 3–7 (1965). [CrossRef]
25. K. Karkkainen and M. Stuchly, “Frequency selective surface as a polarization transformer,” Proc. Inst. Elect Eng. Microw. Antennas Propag. 149(5-6), 248–252 (2002). [CrossRef]
26. J. Hao, Y. Yuan, L. Ran, T. Jiang, J. A. Kong, C. T. Chan, and L. Zhou, “Manipulating electromagnetic wave polarizations by anisotropic metamaterials,” Phys. Rev. Lett . 99, 063908, 1–4 (2007).
27. J. M. Hao, and Lei Zhou, “Electromagnetic wave scatterings by anisotropic metamaterials: Generalized 4x4 transfer-matrix method,” Phys. Rev. B 77, 094201, 1–12 (2008).
28. J. Y. Chin, J. N. Gollub, J. J. Mock, R. P. Liu, C. Harrison, D. R. Smith, and T. J. Cui, “An efficient broadband metamaterial wave retarder,” Opt. Express 17(9), 7640–7647 (2009). [CrossRef] [PubMed]
29. A. C. Strikwerda, K. Fan, H. Tao, D. V. Pilon, X. Zhang, and R. D. Averitt, “Comparison of birefringent electric split-ring resonator and meanderline structures as quarter-wave plates at terahertz frequencies,” Opt. Express 17(1), 136–149 (2009). [CrossRef] [PubMed]
30. J. Hao, Q. Ren, Z. An, X. Huang, Z. Chen, M. Qiu, and L. Zhou, “Optical metamaterial for polarization control,” Phys. Rev. A 80(2), 023807 (2009). [CrossRef]
32. M. Euler, V. Fusco, R. Cahill, and R. Dickie, “325 GHz single layer sub-millimeter wave FSS based split slot ring linear to circular polarization converter,” IEEE Trans. Antenn. Propag. 58(7), 2457–2459 (2010). [CrossRef]
34. E. Doumanis, G. Goussetis, J. L. Gomez-Tornero, R. Cahill, and V. Fusco, “Anisotropic impedance surfaces for linear to circular polarization conversion,” IEEE Trans. Antenn. Propag. 60(1), 212–219 (2012). [CrossRef]
35. A. B. Khanikaev, S. H. Mousavi, C. Wu, N. Dabidian, K. B. Alici, and G. Shvets, “Electromagnetically induced polarization conversion,” Opt. Commun. 285(16), 3423–3427 (2012). [CrossRef]
37. H.-T. Chen, J. F. O'Hara, A. K. Azad, A. J. Taylor, R. D. Averitt, D. B. Shrekenhamer, and W. J. Padilla, “Experimental demonstration of frequency-agile terahertz metamaterials,” Nat. Photonics 2(5), 295–298 (2008). [CrossRef]
38. B. Zhu, Y. Feng, J. Zhao, C. Huang, and T. Jiang, “Switchable metamaterial reflector/absorber for different polarized electromagnetic waves,” Appl. Phys. Lett. 97(5), 051906 (2010). [CrossRef]
39. W. Withayachumnankul, C. Fumeaux, and D. Abbott, “Planar array of electric-LC resonators with broadband tunability,” IEEE Antennas Wirel. Propag. Lett. 10, 577–580 (2011). [CrossRef]
42. M. J. Dicken, K. Aydin, I. M. Pryce, L. A. Sweatlock, E. M. Boyd, S. Walavalkar, J. Ma, and H. A. Atwater, “Frequency tunable near-infrared metamaterials based on VO2 phase transition,” Opt. Express 17(20), 18330–18339 (2009). [CrossRef] [PubMed]
43. D. H. Werner, T. S. Mayer, C. Rivero-Baleine, N. Podraza, K. Richardson, J. Turpin, A. Pogrebnyakov, J. D. Musgraves, J. A. Bossard, H. J. Shin, R. Muise, S. Rogers, and J. D. Johnson, “Adaptive phase change metamaterials for infrared aperture control,” Proc. SPIE 8165, 1–9 (2011). [CrossRef]